6. MARINE BIOF’ILMS ON STAINLESS STEELS: EFFECTS ON
THE CORROSION BEHAVIOUR D. F&on and I. Dupont
CEA-CEREM,Service de la Corrosion,d’Electrochimie et de Chimie des Fluides B.P.6, 92 260 Fontenay-am-Roses,France
Stainless steels are widely used in marine environments, particularly in power plants and in offshore industries. Stainless steel surfaces exposed to natural seawater, are covered in a
short time with an organic and biological layer, called a ‘biofilm’. This biofilm settlement on these surfaces is often divided into at least three main periods: (i) an induction phase during which chemical adsorption of organic chemicals may occur on stainless steel surfaces and also the first adhesion of few bacteria, (ii) a second period corresponding to
an increase in the number of adhesive micro-organisms, and (iii) a third period, a pseudostationary phase, during which the biofilm thickness is more or less constant (bacterial development and detachment). Adhesion of large marine organisms such as mussels, occurs during or after this last third period.
In the last decade, it has been shown by several laboratories that the open-circuit potential of stainless steels is shifted towards the noble direction for stainless steels exposed to natural seawaters during this biofilm formation and development“’. This increase in the corrosion potential of stainless steels in natural seawaters is a major point in explaining the corrosion behaviour in seawater and mainly the localised corrosion which is promoted by potential ennoblement. Our purpose is to focus on this potential ennoblement and consider the questions:
does it appear at the beginning of the biofilm formation br when the biofilm settlement is
Developments in Marine Corrosion
achieved, what is the influence of the steel grade and the environmental conditions (seawater flow rate, temperature,)? 2. EXPERIMENTAL DETAILS 2.1
Materials Eleven different stainless si el grades of Europ an production were used during the
reported tests. They include mainly high-grade materials: austenitic and duplex steels containing h m 2% to 6% molybdenum (Table 1). Specimens included mainly tubes (diameter 23/25 mm, length 1OOmm) and plates (60 x 60 x 3 mm or 200 x 300 x 3 mm).
Table 1 Chemical composition of tested stainless steels (weight %, baIance with Fe)
S A N 28
(1) : several heats tested Stainless steels were used as received. Before exposure, all the specimens were only degreased and then pickled at ambient temperature during 20 minutes in a solution containing 20%HNO, and 2%HF.
Marine Biofilms on Stainless Steels: Effectson the Corroswn Behaviour
Exposure Conditions All reported tests were performed at the CEA seawater facility, called the SlRIUS
facility, which is located at La Hague (Normandy, France). The seawater was pumped at high tide on the rocky coast. The volume of the reservoirs was 120 m3 maximum. There was no light between the pumping system in the sea and the exposed coupons. In the SIFUUS facility, the seawater was heated by a series of heat exchangers and was completely renewed via a single pass loop, no recirculation of the seawater occured. The seawater flowed at 1.5 m3 k' inside the stainless steel tubes (1 m s-') and inside the titanium autoclaves (0.01m d).When titanium autoclaves were used, seawater was heated to 40°C in 15 minutes, but when there was no autoclaves, the time to heat seawater to 40°C was less than two minutes.
Measurements The free corrosion potential of tubes and plates was measured versus the saturated
calomel electrode (SCE) every hour by means of a Solartron Schlumberger data acquisition system (3351 D, ORION). Galvanic currents were also recoded every hour with the same device: the measurements are performed using an external resistance of 10
ohms for each galvanic couple (tubes or plates). Seawater temperatures, pH, redox potentials (platinum potential versus SCE) were also recorded every hour. Chemical analyses of the seawater were also performed during the tests: they include the main cations and anions, dissolved oxygen, total conductivity, organic matter content and chlorophyll a. Mean values obtained during the reported tests are shown on Table 2: no major variations were observed, except the ambient temperatures of the seawater which varied fiom 7°C in winter up to 17 "C in summer.
Developments in Marine Corrosion
Table 2 Seawater main composition during the reported tests (mean values with standard deviation)
mg kg-l mg k g '
_ _ _ 904 L _ _ _ 904 L
MO SM 0
...... 316 L ......316 L
18 T i m e (days)
Figure 1 Evolution of the corrosionpotentials of stainless steels in natural seawater at ambient temperature
Marine BiqfiIm on Stainless Steels: Effectson the Corrosion Behaviour
Figure 2 Evolution of the corrosionpotentials of 316Lplates in natural seawater (dash lines :no cowosion on 31 6L coupons, continuous line :crevice corrosion on the coupon)
Figure 3 Season influence on the evolution of the corrosionpotential of Stainless steels (654 SMO)plates in natural seawater at ambient temperature
3. RESULTS AND DISCUSSION 3.1
Free Corrosion Potential Measurements Figure 1 illustrates the evolution of the fiee corrosion potentials (ECom)of stainless
steel coupons when they are exposed to natural seawater at ambient temperature. Three main periods are observed whatever is the season or the grade of stainless steel. A first
Developments in Marine Corrosion
period during which E,,
is nearly constant at a low value (-100 to -300 mV vs. SCE) and
which lasts between 40 to 150 hours in our experimental conditions. This first period will be called the ((incubationN period below. Then the increase of Eco, takes place during about 100 hours. The third and last period corresponds to a constant EComat 300 f 50 mV
vs. SCE with relatively small variations, even after 3000 hours of exposure (maximum exposure time of our experiments). 3.1.1 Effect of sfainless steel grade. At ambient temperature, the potential
ennoblement occurs with all tested stainless steel grades: 316L, 904L, URANUS B26, SB8,47N and 52N, SAF 2507 and 2205, AVESTA 654 SMO and 254 SMO, S A N 28. No differences are observed in terms of time to reach the maximum potential or values of this maximum potential. This result is illustrated in Figure 1 where the E,,
evolution of 316L,
904L and 254 SMO are compared in natural seawater at ambient temperature. If corrosion occurs during the exposure, the potential of the corroded coupons does not increase as described above and may decrease as illustrated in Figure 2 where a 3 16L coupon suffers crevice corrosion after 7 to 8 days of exposure to natural flowing seawater at ambient temperature. 3.1.2 Seasonal influence. Exposure of 654
SMO tubes and plates have been
performed in spring, summer, autumn and winter. As shown in Figure 3, the incubation period varies from 40 hours in summer (mean seawater ambient temperature : 17.4"C)to some 110 hours in winter (mean seawater ambient temperature : 8.7"C) for stainless steel plates. In spring and autumn, the incubation time is between these two extreme values. But the maximum E,,
values are the same whatever is the season, about 300 mV vs. SCE
under our experimental conditions. 3.1.3 Coupon influence. Two types of stainless steel coupons were used, as
previously reported: plates and tubes. The same evolution and the same maximum values of ECor were obtained on plates and tubes. But the incubation times were always longer for tubes (some 10 hours following the exposure conditions, mainly the season). This difference is probably due to the seawater flow which was low on plates (about 0.01 m s-') and higher in tubes (1 m d).
Marine B W J h on Skainless Steels: Effectson the Corrosion Behaviour
6 cn_ >
Figure 4 Free corrosion potential evolution of stainless steel (654 SMO) tubes in flowing natural seawater (I m.s-9 at 2OoC,30°C and 40°C 3.1.4 Eflect of temperature. Experiments were conducted at the SIRIUS facility,
at three temperatures, with twenty 654 SMO tubes at each temperature. Free corrosion potential evolutions are illustrated by the Figure 4 for these tubes and may be smarised
as follows. At 20°C and 30"C, previous results obtained at ambient temperature are confirmed with a rapid increase in the corrosion potentials of the stainless steel tubes up to
+300 mV vs. SCE in about 10 to 12 days. At 4OoC, the free corrosion potential of all the tested stainless steel tubes remains constant at about -100 mV vs. SCE which is the starting value of the potentials at 20°C and 30°C. Electrode potential ennoblement occurs also on platinum and titanium. At 20"C, titanium E ,,,
values reach -250 mV vs. SCE after 30 days of exposure, at 30"C, they
reach -150 mV vs. SCE but at 4OoC, titanium,,E
is nearly constant (%lomV vs. SCE
after 30 days of exposure). On platinum, high potential values (270 to 300 mV vs. SCE) are obtained whatever the temperature is, while the starting values of the redox potentials are nearly the same at 20,30, or 40°C: between 100 and 200 mV vs. SCE.
In another series of tests, five superaustenitictubes are exposed to seawater heated at 30°C and five other tubes are located in the section where the same seawater is cooled at 26°C after being heated up to 4OOC. The,,E
evolution of these tubes is the following: at
Developments in Marine Corrosion
both temperatures, with seawater heated to 30°C or with seawater cooled from 40°C to 25"C, there is an increase of E., "enough" to avoid E,
A temporary heating to 40°C does not alter seawater
3.2 Electrochemical Investigations 3.2.1 Galvanic currents. Stainless steel and carbon steel specimens have been
coupled as described above, and the coupled current have been followed. In all cases, an important increase in the galvanic current (stainless steel is cathodic and carbon steel anodic) is observed as shown in Figure 5 where the observed evolution of the galvanic current is reported for three seasons : winter, spring and summer. Figure 6 shows that the galvanic current increase after a longer incubation time in winter (350 hours) than in summer (120 hours), in accordance with the E,
evolutions. It could mean that the
cathodic properties of the stainless steel are affected by the biofilm formation at ambient temperatures, in natural seawater. 3.2.2Polarisation currents. Stainless steel plates (AVESTA 254 SMO)have been
polarised at plus and minus 20 mV around E,, ,during their exposure to natural seawaters at ambient temperature. The polarisation current is the current which is needed to polarise
,, the specimen o f f 20 mV vs. E
Before the EcOrincrease, the polarisation currents are
constant between 5 and 10 pA cm.' (EGO,between -200 and -150 mV vs. SCE). The polarisation currents reach 20 to 40 pA cm-2when the stainless steel ennoblement takes place (E,,,
increases to +250 mV vs. SCE). This increase in the polarisation current which
takes place with an increase in the corrosion potential of the stainless steel, means that it is the cathodic reaction (oxygen reduction in the case of aerated seawater) on stainless steels which is faster or which is replaced by a faster cathodic reaction when biofilm formation occurs at ambient temperatures in natural seawater. 3.2.3 Oxygen influence. The influence of oxygen has been checked during one
experiment where deaerated seawater was used at ambient temperature. The stainless steels E,
were found to be constant between -100 and 0 mV vs.SCE during the tests as
shown in Figure 6: no stainless steel ennoblement occurs without oxygen. This result points out the importance of oxygen in the ennoblement process.
Marine Biofilms on Stainless Steels: Effectson the Corrosion Behaviour
30 20 10 0 -1 0
Figure 5 Evolution of the current between stainless steel (cathodic) and carbon steel (anodic) exposed to natural seawater (coupling current in p A cm-2, anodic and cathodic areas are the same) 3.3 Bioiilm Settlement
3.3.1 Masses of biofilm. Sampling of biofilms were perfonned on exposed coupons and the first investigations were performed on the biofilm masses. In fact, the biofilm masses were always very low at the beginning of the seawater exposure: less than 0.1 mg cm-', when the fiee corrosion potentials of the stainless steel coupons are lower than 200
mV vs. SCE, on coupons exposed at ambient temperature. Generally speaking, biofilm masses increased with exposure time, so with Em,.,at the beginning of exposure. But, as
shown in Table 3 where are reported the biofilm masses collected on tubes exposed in natural flowing seawater at 20,30and 40"C, biofilms are present on all the stainless steel tubes, including studies at 40°C. The fact that there is no , E
increase at 40"C, in spite of
a massive presence of biofilm, clearly demonstrates that biofilm settlement is possible in seawater without ennoblement of stainless steel.
Developmentsin Marine Corrosion
3.3.2 SEM observations. Biofilm observations were performed with a Scanning Electron Microscope on stainless steel coupons, at different values of Ecom A special preparation of the samples was performed, including biofilm fixation with glutarhaldehyde,dehydration and metallization. In fact, no microorganismswere observed by SEM on stainless steel surfaces when E,
is lower than 200 mV vs. SCE. At higher
potentials (EC0>250 mV vs. SCE), few microorganisms (bacteria shape) are seen on stainless steel coupons: about lo5 bacteria per cm2 after 360 hours of exposure in natural seawater at ambient temperature during the winter test (Ecom= 253 mV vs. SCE). So it seems that the ennoblement of stainless steel occurs before bacteria settlement on stainless steel surfaces could be observed by SEM. To be more precise, and as far as bacteria observed by SEM could be considered asirreversibly adhesive (ennoblement occurs before the irreversible adhesion of bacteria on the surfaces under our experimental conditions).
T l m c (bourr)
Figure 6 Evolution of stainless steel (316L) potentials in aerated and deaerated seawater
Marine B W $ h on Stainless Steels: Effects on the Corrosion Behaviour
Table 3 Biojlm settlement on stainless steel mt$aces exposed to natural seawater (Epijluorescence observationsof the percentages of the stainless steel surface covered with bacteria)
Table 4 Biofirm sampling on stainless steel tubes exposed to seawater thermally altered
Potential vs. SCWmV 25
Wet biofilm content
t 27days 7days
Developments in Marine Corrosion
3.3.3 Direct epifluorescence observations. More infomation on the biofilm
settlement have been obtained by direct epifluorescence on exposed stainless steel surfaces. This technique allows one to count the total number of bacteria which colonise a surface, whatever is the adhesion of bacteria on this surface, reversible or irreversible. During experiments performed on the SIRIUS facility, the direct observations of microorganisms on surfaces by epifluorescence show that bacteria are gathered and numerous on stainless steel surfaces, and so difficult to count, even at the beginning of exposure. In a first attempt, the biofilm settlement on the surfaces is evaluated by the percentage of the surface covered by microorganisms (dead or alive) and eventually by substances which react also with the fluorescent substance (DAPI). These observations are performed at different exposure times and at different EComvalues. The results obtained on coupons exposed at 20°C and at 40°C are summarized in Table 4. They show clearly that the percentage of the surfaces covered by microorganisms is the same or even more important at 40°C than at 20°C whereas the free corrosion potential at 40°C stays constant and increases at 2OOC. It shows clearly that the presence of a biofilm and bacteria on surfaces does not involve by itself the potential ennoblement. 3.3.4 Microbiological investigations. Investigations are then performed on the
number of bacteria which are present in the biofilm to determine if there is a major difference between the bacterial colonization at 20°C and at 40°C which may explain the electrochemical behaviours. Aerobic, facultative anaerobic and strict anaerobic bacteria are isolated and counted. As shown in Table 5 , there is no major difference between the number of bacterial populations, whatever the counting method. The potential ennoblement observed on stainless steel surfaces at 20°C could not be explained only by the presence of bacteria on stainless steel surfaces: there is no differences concerning the global parameters of surface colonization (mass of biofilm, percentage of covered surface by the biofilm, total number of bacteria or number of aerobic, anaerobic or facultative bacteria) between 20°C and 40OC; the potential of stainless steel becomes more positive at 20°C but not at 40°C.
Marine Bioflms on Stainless Steels: Effectson the Corroswn Behaviour
Table 5 Number of bacteria on stainless steel sufaces (200 hours of seawater exposure) Total
Free corrosion number of (bacterialcm2) bacteria
4.4 x lo7 6.0
3.3 x lo7
The noble shift in the free corrosion potential of stainless steels in natural seawater occurs at ambient temperatures, 20°C and 30°C under our experimental conditions and is observed for all the other tested stainless steels: 654 SMO,254 SMO,SAF 2507 and 2205, S A N 28,
URANUS B26, SB8, 47N and 52N, 316L and 904L. The corrosion potentials
rise fiom about -2OO/-100 mV vs. SCE to some +300 f 50 mV vs. SCE. At ambient temperatures, stainless steel ennoblement is promoted in summer, but it occurs also in winter. At 4OoC, the fiee corrosion potentials of stainless steels are constant at about -100 mV vs. SCE while biofilm formation and bacterial settlement on stainless steel surfaces occur at the three tested temperatures. Biofilms developed at the three tested temperatures do not present differences in term of global parameters (masses, bactezial numbers, aerobic and anaerobic bacteria, etc.). Future work will concern the metabolic or the enzymatic activities of the bacteria. The chemical compounds (hydrogen peroxide and organic acids for instance) generated by the metabolic reaction of bacteria may be the key parameters for an explanation for the positive shift in the fiee corrosion potential observed at 20°C and 30°C.
Developments in Marine Corrosion
This work was supported, in part, by the Commission of the European Communities under MAST and STRIDE contracts.
J.P. Audouard et al., Proceedings of the Third EFC WP Microbial Corrosion, Estonl (Portugal), 1995, Paper No. 15 .
J.P. Audouard et al., Proceedings of the International Congress on Microbial Induced Corrosion, New Orleans (Louisina-USA), 1995, Paper No. 3.
A.Mollica and A.Trevis, 4th Int. Congress on Marine Corrosion and Fouling, 1976, Juan-les-Pins, France.
E. Bardal, J.M.Drugli and P.O.Gartland, ,Corrosion Science, 1995,35,(1-4), 257.
P. Chandrasekaran and S.C. Dexter, Corrosion’93 NACE conference, 1993, Paper No. 493.